Langmuir 2004, 20, 9745-9754
Human Serum Albumin Adsorption on TiO2 from Single Protein Solutions and from Plasma S. R. Sousa,*,†,‡,§ P. Moradas-Ferreira,| B. Saramago,⊥ L. Viseu Melo,# and M. A. Barbosa†,‡ Instituto de Engenharia Biome´ dica (INEB), Laborato´ rio Biomateriais, Rua do Campo Alegre, 823, 4150-180 Porto, Portugal, Universidade do Porto, Faculdade de Engenharia, Departamento Engenharia Metalu´ rgica e de Materiais, Rua Dr. Roberto Frias, s/n, 4200-465 Porto, Portugal, Instituto Superior de Engenharia do Porto (ISEP), Departamento Engenharia Quı´mica, Rua Dr. Bernardino de Almeida, 431, 4200-072 Porto, Portugal, Instituto de Biologia Molecular e Celular (IBMC), Grupo de Microbiologia Celular Aplicada, Rua do Campo Alegre, 823, 4150-180 Porto, Portugal, Instituto Superior Te´ cnico (IST), Centro de Quı´mica Estrutural, Avenida Rovisco Pais, 1049-001 Lisboa, Portugal, and Instituto Superior Te´ cnico (IST), Departamento Fı´sica, Avenida Rovisco Pais, 1200 Lisboa, Portugal Received April 1, 2004. In Final Form: July 28, 2004 In the present work, the adsorption of human serum albumin (HSA) on commercially pure titanium with a titanium oxide layer formed in a H2O2 solution (TiO2 cp) and on TiO2 sputtered on Si (TiO2 sp) was analyzed. Adsorption isotherms, kinetic studies, and work of adhesion determinations were carried out. HSA exchangeability was also evaluated. Surface characterization was performed by atomic force microscopy (AFM), X-ray photoelectron spectroscopy (XPS), and wettability studies. The two TiO2 surfaces have very distinct roughnesses, the TiO2 sp having a mean Ra value 14 times smaller than the one of TiO2 cp. XPS analysis revealed consistent peaks representative of TiO2 on sputtered samples as well as on Ti cp substrate after 48 h of H2O2 immersion. Nitrogen was observed as soon as protein was present, while sulfur, present in disulfide bonds in HSA, was observed for concentrations of protein higher than 0.30 mg/mL. The work of adhesion was determined from contact angle measurements. As expected from the surface free energy values, the work of adhesion of HSA solution is higher for the TiO2 cp substrate, the more hydrophilic one, and lower for the TiO2 sp substrate, the more hydrophobic one. The work of adhesion between plasma and the substrates assumed even higher values for the TiO2 cp surface, indicating a greater interaction between the surface and the complex protein solutions. Adsorption studies by radiolabeling of albumin (125I-HSA) suggest that rapid HSA adsorption takes place on both surfaces, reaching a maximum value after ∼60 min of incubation. For the higher HSA concentrations in solution, a multilayer coverage was observed on both substrates. After the adsorption step from single HSA solutions, the exchangeability of adsorbed HSA molecules by HSA in solution was evaluated. The HSA molecules adsorbed on TiO2 sp seem to be more easily exchanged by HSA itself than those adsorbed on TiO2 cp after 24 h. In contrast, after 72 h, nearly all the adsorbed albumin molecules effectively exchange with other albumin molecules.
Introduction At present, several promising multifunctional biomaterials are available that are being applied to new types of artificial organs and advanced medical devices.1 Nevertheless, metals are still the most suitable biomaterials for replacing hard tissue due to good bone matching mechanical properties.2 The physiological inertness of titanium associated with its exceptional mechanical properties and favorable osteointegration makes it available as a replacement for * Corresponding author. Current address: Instituto de Engenharia Biome´dica (INEB), Laborato´rio de Biomateriais, Rua do Campo Alegre, 823, 4150-180 Porto, Portugal. Phone: 351 22 6074985. Fax: 351 22 6074567. E-mail: [email protected]
† Instituto de Engenharia Biome ´ dica (INEB). ‡ Universidade do Porto. § Instituto Superior de Engenharia do Porto (ISEP). | Instituto de Biologia Molecular e Celular (IBMC). ⊥ Instituto Superior Te ´ cnico (IST), Centro de Quı´mica Estrutural. # Instituto Superior Te ´ cnico (IST), Departamento Fı´sica. (1) Nakabayashi, N.; Iwasaki, Y. European white book on fundamental research in materials science; Ru¨hle, M., Dosch, H., Mittemeijer, E. J., Van de Voorde, M. H., Eds.; Max Plank Institut fur Metallforschung: Stuttgart, Germany, 2000; pp 70-71. (2) Windler, M.; Klabunde, R. In Titanium in medicine: Material science, surface science, engineering, biological responses and medical applications; Brunette, D. M., Tengvall, P., Textor, M., Thomsen, P., Eds.; Springer-Verlag: Berlin, Germany, 2001; pp 703-746.
bones and cartilage in a variety of surgeries, namely, orthopedic, dental, spinal, as well as reconstructive and plastic surgery.3 However, the insertion of a foreign material into the human body activates defense mechanisms and triggers the coagulation system when the material is brought into contact with blood. White cells may be recruited to the wound site, with subsequent release of reactive oxygen species such as H2O2 and O2-. It has been reported by Tengvall et al. that Ti forms stable Ti-peroxy complexes in the presence of large amounts of H2O2.4 The differential response of tissue to implanted materials may arise mainly from differences in the adsorption of proteins.5 The organization of the adsorbed proteins depends on the type of the surface, since proteins display different relative affinities for different surfaces. Consequently, since each cell type has a different set of specific receptors for proteins, the efficiency of cell attachment, proliferation, and viability is dependent on surface parameters, namely, oxide composition, surface (3) Larsson, C.; Esposito, M.; Liao, H.; Thomsen, P. In Titanium in medicine: Material science, surface science, engineering, biological responses and medical applications; Brunette, D. M., Tengvall, P., Textor, M., Thomsen, P., Eds.; Springer-Verlag: Berlin, Germany, 2001; pp 587-648. (4) Tengvall, P.; Lundstrom, I. Clin. Mater. 1992, 9, 115-134. (5) Ostumi, E.; Chapman, R. G.; Liang, M. N.; Meluleni, G.; Pier, G.; Ingberg, D. E.; Whitesides, G. M. Langmuir 2001, 17, 6336-6343.
10.1021/la049158d CCC: $27.50 © 2004 American Chemical Society Published on Web 09/23/2004
Langmuir, Vol. 20, No. 22, 2004
roughness, surface charge, and contaminants, among other characteristics. This work aimed at assessing albumin adsorption on two different surfaces, TiO2 sputtered on Si (TiO2 sp) and TiO2 formed on commercially pure titanium after H2O2 immersion (TiO2 cp). The objective was to have titanium oxide chemically similar to those used in clinical practice, stable with two different roughnesses. The protein solutions were human serum albumin (HSA) and plasma. Surfaces were characterized using atomic force microscopy (AFM), imaging and roughness analysis, X-ray photoelectron spectroscopy (XPS), and wettability studies, leading to the surface free energy. The adsorption kinetics and isotherms were evaluated by two different techniques, radiolabeling of albumin (125I-HSA) and XPS. With the latter technique, it was possible to follow albumin adsorption in TiO2 through the increase of nitrogen and carbon groups and the decrease of titanium and oxygen intensity. The work of adhesion between protein solutions and TiO2 substrates was evaluated through wettabilitty studies. HSA exchangeability was also estimated by 125IHSA. Materials and Methods TiO2 Substrates. Commercially pure titanium sheets, 1 mm thick, were used. The nominal composition (wt %, max) was the following: 0.20 Fe, 0.05 N, 0.08 C, and 0.015 H. The surface was roughened by chemical polishing (cp) with an etching acid solution (2:3 parts by volume, 40% HF + 60% HNO3 (v/v)) for 30 s. The substrates were preincubated in 10 mM H2O2 for 48 h to obtain a regular titanium oxide film. TiO2 sputtered substrates were prepared using an automated, load locked ion beam deposition system (Nordiko N3000), which is described elsewhere.6 The TiO2 films (50 nm) were deposited on Si wafers (polished/ etched, crystal orientation 〈100〉, from AUREL Gmbh) by ion beam sputtering from a Ti cp target, in the presence of a mixed Ar-O2 beam coming from the assist gun (15.02% O2 in Ar). The deposition rate was 0.038 nm/s. An acceleration voltage of +1450 V (33 mA Xe beam, 1 sccm Xe, 110W RF plasma) and an extraction voltage of -300 V were used at the deposition gun. The Ar-O2 beam was created by accelerating the plasma inside the assist gun with +200 V (15 mA beam, 10 sccm Ar-O2, 50W RF plasma) and using an extraction voltage of -100 V. The pressure during the assisted deposition was 1.3 × 10-4 Torr. A filamentless neutralizer (40 mA, 3 sccm Ar-O2) next to the ion source avoided surface charging during the dielectric deposition. The wafers were diced into pieces (5 × 5 µm2) using a DISCO DAD321 automated saw. Before dicing, all wafers were coated with 1.5 µm of photoresist (reference PFR7790EG, from JSR Electronics), to protect the film surface. Just before being used, the TiO2 sputtered films were cleaned twice in acetone and immersed in a “piranha” solution (7:3 parts by volume, 98% H2SO4 + 30% H2O2 (v/v)) for 90 s (caution: this solution reacts violently with many organic materials and should be handled with great care). Substrates were washed in ethanol, water (distilled and deionized), and again in ethanol for 2 min in an ultrasonic bath. Protein Solutions. Human serum albumin (Sigma, ref A1653) solutions were prepared in phosphate buffered saline (PBS, Sigma, pH 7.4, ref P-3813) at concentrations of 0.2, 0.4, 1.0, 4.0, and 10.0 mg/mL. Plasma was obtained from healthy blood donors from the Portuguese Blood Institute (IPS). The concentrations used were 100 and 10% (v/v). The water used was distilled and deionized with a resistivity of >16 MΩ cm. Atomic Force Microscopy (AFM). Surface morphology and roughness were determined using a commercial atomic force (6) Gehanno, V.; Freitas, P. P.; Ferreira, J.; Almeida, B.; Sousa, J. B.; Kling, A.; Soares, J. C.; Silva, M. F. IEEE Trans. Magn. 1999, 35, 4361-4367.
Sousa et al. microscope (Digital Instruments Nanoscope). The instrument was operated in tapping mode, and the sizes of the images were 1 × 1 µm2. Three samples of each type were analyzed at a randomly chosen location. The surface roughness was obtained from scanned areas of 1000 × 1000 nm2. To characterize the roughness, the average roughness (Ra) was obtained as well as the standard deviation of the amplitude (Rq) and the maximum peak (Rmax). X-ray Photoelectron Spectroscopy (XPS). XPS measurements were carried out on a VG Scientific ESCALAB 200A (U.K.) spectrometer using Mg KR (1253.6 eV) as a radiation source. The photoelectrons were analyzed at two takeoff angles, 0 and 60°. Survey XPS spectra were acquired from 0 to 1100 eV before and after hydrogen peroxide treatment as well as after protein adsorption. High-resolution spectra for Ti2p, O1s, C1s, N1s, and S1s were also obtained. Elemental atomic percentages of Ti, O, C, N, and S were determined after deconvolution of the highresolution spectra, using an XPS peak-fitting program (XPS PEAK, version 4.1). To take into account shifts caused by charging of the sample surface, all spectra were adjusted taking the C1s peak at 285.0 eV as the reference for the adventitious carbon contamination. The elemental atomic percentages of Ti, O, C, N, and S were determined for adsorption times of 5, 10, 30, 60, and 360 min at HSA concentrations of 0.20 and 4.0 mg/mL (kinetics) and, after 60 min of HSA adsorption, as a function of HSA concentration in the range 0.20-4.0 mg/mL (adsorption isotherms). Wettability Studies. Contact angle measurements were performed with a contact angle measuring system from Data Physics, model OCA 15, equipped with a video charge-coupled device (CCD) camera and SCA 20 software. The equipment incorporates an electronic syringe unit with a gastight 500 µL dosing syringe (Hamilton). Contact angles were obtained by the sessile drop method, at 25 °C in a chamber saturated with the liquid sample. The drop was recorded as soon as stabilization was achieved, and images were recorded every 2 s for up to 600 s. Digital images of the drop were acquired by the CCD camera and used for the calculation of the contact angle. For the contact angle determination, an ellipse function was fitted to the measured contour line, obtaining the best accuracy. The contact angle value was extrapolated to t ) 0 s for water and to t ) 600 s for protein solutions, using a curve-fitting program. In each experiment, at least 10 drops of ∼4 µL were used. Surface tension of the protein solution in equilibrium with its own vapor (γLV) was obtained through the analysis of the shape of a pendant drop kept at 25 °C in a chamber saturated with the liquid sample. As drop stabilization was achieved, images were taken every 2 s for 600 s. In each experiment, at least 10 drops of ∼20 µL were analyzed. The liquid densities at 25 °C were determined using an Anton Paar density meter. Surface free energy of all types of titanium was assessed by the Owens-Wendt-Rabel-Kaelble7 (OWRK) method using as testing liquids distilled and deionized water and diiodomethane (>99%, from Sigma-Aldrich). The polar and dispersive components of the surface tension of the liquids at 25 °C were estimated from the correspondent values at 20 °C, taken from the literature8 [γLV of water and diiodomethane: 71.52 ( 0.13 mN/m (γd ) 21.42 mN/m; γp ) 50.11 mN/m) and 50.46 ( 0.07 mN/m (γd ) 50.46 mN/m; γp ) 0 mN/m), respectively]. The estimation was based on the assumption that the ratio between the dispersive and polar components of the liquid surface tension did not vary with the temperature. This determination was based on Young’s equation which relates the surface tension of a liquid in equilibrium with its vapor (γLV) with the contact angle (θ) of the same liquid drop on the surface of an ideally smooth flat solid. The difference γSV γSL can be obtained from Young’s equation and experimentally measured values of γLV and θ. (7) Owens, D. K.; Wendt, R. C. J. Appl. Polym. Sci. 1969, 13, 17411747. (8) Kerkeb, M. L.; Gonza´lez-Caballero, F.; Chibowski, E. J. Colloid Interface Sci. 1993, 159, 439-443.
HSA Adsorption on TiO2
Langmuir, Vol. 20, No. 22, 2004 9747
The work of adhesion (the negative part of the Gibbs energy of adhesion) for a liquid in contact with a solid (W) may be obtained by the Young-Dupre´ equation:
W ) γLV + γSV - γSL ) γLV(1 + cos θ)
The interfacial free energy between the solid and the liquid can be calculated, according to Owens and Wendt,7 considering that the total surface free energy is expressed as a sum of two components arising from dispersive and polar contributions (γd and γp, respectively). Assuming further the geometric mean approach, for the polar and dispersive components of the work of adhesion, the solid-liquid interfacial free energy may be written as:
γSL ) γSV + γLV - 2xγdSVγdLV - 2xγpSVγpLV
d ) and polar (γpSV) components can γSV as well as the dispersive (γSV be calculated from Young’s equation and eq 2 using experimental values of contact angles measured with a pair of testing liquids with known polar and dispersive components. Protein Quantification by Radioactivity. Quantification of albumin adsorbed on the TiO2 surface was performed using 125I-labeled albumin. Human plasma albumin (Sigma) was labeled with 125I using the Iodogen method.9,10 125I-HSA was passed through a Sephadex G-25 M column (PD-10 column, from Amersham Pharmacia Biotech) to remove unbound 125I. The yield of iodination was always higher than 98%, as determined by precipitating the 125Ilabeled albumin with 20% trichloroacetic acid (the TCA method). Several authors reported11-13 that some measured amounts of adsorbed protein were erroneously high due to interactions of residual free 125I ions, present in the protein solution, with metal surfaces. The contribution of free 125I to the total radioactivity found on the metal surfaces was estimated using unlabeled albumin solutions at a concentration of 1.0 mg/mL and an amount of free 125I ions equivalent to that present as free 125I ions in the labeled protein solutions. In all studies in which radiolabeling methods are used, it must be kept in mind that the behavior of the labeled protein may or may not reflect the behavior of unlabeled protein.14 To assess if preferential adsorption of 125I-labeled albumin occurred on TiO2 surfaces, a series of control experiments were performed varying the ratio of labeled to unlabeled albumin (10-50%). The final concentration of the albumin solutions (1.0 mg/mL) was confirmed by the bicinchoninic acid (BCA) assay using a BCA assay kit from Pierce and bovine serum albumin (BSA) as the standard.15 Protein solutions for the adsorption experiments were prepared by adding 125I-HSA to unlabeled albumin solution to obtain a final activity of ∼108 cpm/mg. HSA adsorption tests were performed by placing the Ti substrates in a 24-well tissue plate (Sarsted). A drop of 10 µL of 125I-HSA solution was added onto each surface. To avoid evaporation, PBS was added to the wells in the periphery. Adsorption tests were carried out at 25 °C over a period of 60 min. After this period, the drop was absorbed from the surface with absorbent paper and the surface was washed three times with PBS. The samples were transferred to radioimmunoassay tubes, and surface activity was measured using a gamma counter. All experiments were done in triplicate. The counts from each
(9) Iodine-125, A guide to radioiodination techniques; Amersham Life Science: Little Chalfont, Buckinghamshire, U.K., 1993; p 64. (10) Lima, J.; Sousa, S. R.; Ferreira, A.; Barbosa, M. A. J. Biomed. Mater. Res. 2001, 55, 45-53. (11) Williams, D. F.; Askill, I. N.; Smith, R. J. Biomed. Mater. Res. 1985, 19, 313-320. (12) Sheardown, H.; Cornelius, R. M.; Brash, J. L. Colloids Surf., B 1997, 10, 29-33. (13) Du, Y. J.; Cornelius, R. M.; Brash, J. L. Colloids Surf. 2000, 17, 59-67. (14) Yu, X. J.; Brash, J. L. In Test procedures for the blood compatibility of biomaterials; Dawids, S., Ed.; Kluwer Academic Publishers: Dordrecht, The Netherlands, 1993; pp 287-330. (15) Smith, P. K.; Krohn, R. I.; Hermanson, G. T.; Mallia, A. K.; Gartner, F. H.; Provenzano, M. D.; Fujimoto, E. K.; Goeke, N. M.; Olson, B. J.; Klenk, D. C. Anal. Biochem. 1985, 150, 76-85.
sample were averaged, and the surface concentration was calculated by the following equation:
HSA (mg/m2) )
counts (cpm) × [HSA]solution (mg/mL) Asolution(cpm/mL) × SA (m2)
where the counts measure the radioactivity of the samples, [HSA]solution is the albumin concentration solution, Asolution is the specific activity of the albumin solution, and SA is the surface area. To understand albumin adsorption on titanium oxide substrates, the kinetics of adsorption of HSA for concentrations of 0.20 and 4.0 mg/mL (during periods of 5, 30, and 60 min) and adsorption isotherms were investigated in an HSA concentration range of 0.20-10.0 mg/mL. Displacement tests were carried out by immersing the labeled Ti surface over 24 and 72 h in an unlabeled HSA pure solution (exchange). The substrates were washed three times with PBS, and the residual activity was counted. Statistical analysis of the experimental results was performed using the Kurskall-Wallis, nonparametric tests.
Results Surface Characterization. AFM. To assess the binding of proteins, namely, albumin to titanium, surfaces were first characterized for roughness and morphology using AFM. The surface roughnesses of the various Ti surfaces are presented in Table 1. When treated with hydrogen peroxide, a slight increase in surface roughness at the nanometric scale (Ra, Rq, and Rmax values) was observed, leading to a more uniform surface. This effect is probably related to the strong oxidizing effect of H2O2. Figure 1 shows the 3D AFM images of all Ti surfaces. The increased roughness introduced by hydrogen peroxide treatment is evident in Figure 1b and c for the cp substrate. The two TiO2 surfaces have distinct roughnesses, with the TiO2 sp having a mean Ra value 14 times smaller than the one for the TiO2 cp (Table 1). XPS. Titanium surfaces were characterized by XPS to explore the detailed surface chemistry after different surface modifications. To check the presence of additional elements than those expected (Ti, O, and contaminant C), wide scans were performed in all Ti samples before protein adsorption. N and Ca were detected as traces, arising from the manufacture of titanium. For the TiO2 cp substrates, N results from the HNO3 initial treatment. The spectra of all the elements detected are identical for TiO2 sp and TiO2 cp surfaces. Analysis of fitted XPS high-resolution spectra allows characterization of the chemical environment of the different elements. To obtain a regular and uniform layer of TiO2, several surface treatments of Ti cp were tried: exposure to air (48 h) and immersion in 10 mM H2O2 and in 100 mM H2O2 for two different periods of time, 24 and 48 h. Two angles of escape, 0 and 60° (XPS) were used. The high-resolution O1s spectra obtained from TiO2 cp with several surface treatments showed a shoulder on the higher binding energy side, justifying the separation of the O1s spectrum into two components. The binding energy (BE) assigned to titanium oxide (OM) (530.4 eV)16,17 appears in the low-energy range followed by other components at higher BEs, namely, hydroxide/hydroxyl (16) Shirkhanzadeh, M. J. Mater. Sci.: Mater. Med. 1995, 6, 206210. (17) Kilpadi, D. V.; Raikar, G. N.; Liu, J.; Lemons, J. E.; Vohra, Y.; Gregory, J. C. J. Biomed. Mater. Res. 1998, 40, 646-659.
Langmuir, Vol. 20, No. 22, 2004
Sousa et al.
Table 1. Ra, Rq, and Rmax Values for All the Ti Substrates Studieda
TiO2 sp Ti cp (before H2O2 treatment) TiO2 cp (after H2O2 treatment)
0.23 (0.22, 0.29) 4.75 (4.4, 6.3) 5.15 (5.0, 6.6)
0.29 (0.29, 0.36) 6.50 (5.7, 8.1) 6.53 (6.3, 8.7)
2.75 (2.7, 3.7) 55.1 (53, 59) 52.9 (52, 67)
The first and third quartiles are shown in parentheses.
groups plus chemisorbed water (OH) (532.2 eV).17,18 Armstrong et al.19,20 found that binding energy differences between two major transitions may indicate the chemical composition of a metal oxide. The BE difference between the O1s and Ti2p3 peaks is ∆BE ) O (1s) - Ti (2p/3) ) 71.5 eV, which, according to the data obtained by the same authors, corresponds to TiO2. The Ti2p peak obtained at 60° was a doublet peak, Ti2p3/2 at 458.9 eV and Ti2p1/2 at 464.4 eV for Ti cp surfaces exposed to air, revealing a Ti4+ oxide state,21,22 whereas that obtained at 0° additionally showed metallic-state titanium (453.7 eV).21-23 This suggests that the surface film is not thick enough for photoelectrons from the bulk metal to reach the surface and that the Ti oxide film surface consists essentially of TiO2, without suboxides such as TiO and Ti2O3. After 24 h of 10 mM H2O2 treatment, Ti (0) is still observed at a takeoff angle of 0° and at 60°, TiO2 constitutes the oxide with a layer of hydration groups as it was observed for the O1s spectra at 532.2 eV. Both hydrogen peroxide treatments (48 h, 10 and 100 mM) lead to the formation of a thicker TiO2 layer harboring hydration groups, as indicated from both 0 and 60° measurements. The Ti/OM ratio, 0.55 and 0.52 at takeoff angles of 0 and 60°, respectively, for the 10 mM H2O2 treatment was closer to the theoretical value for TiO2. Therefore, this treatment was selected to be applied in all the Ti cp specimens. The C1s spectra can be resolved in two different peaks: one at 285.0 eV representing carbons in a hydrocarbontype environment (sCH3, sCH2s) and the other one at 288.9 eV representing carbons in a sCsFs bond or s CdO, originated by the chemical etching.24 Nitrogen is always present as a trace element with one peak centered at 400.9 eV characteristic of -NH- bonds.25 The Ca spectra present a doublet peak with Ca2p3/2 at 347.2 eV and Ca2p1/2 at 350.7 eV. The BEs suggest that a CaO or CaCO326,27 compound may be present at the surface. Ca is a trace element of Ti. Wettability Studies. To obtain further data on the surface characteristics, the surface free energy was evaluated. The values of the contact angles of water and diiodomethane for the TiO2 substrates (Table 2) were obtained by extrapolation of time-dependent experimental results to t ) 0 s. (18) Lausmaa, J.; Kasemo, B.; Mattsson, H. Appl. Surf. Sci. 1990, 44, 133-146. (19) Armstrong, N. R.; Quinn, R. K. Surf. Sci. 1977, 67, 451-468. (20) Leitao, E.; Barbosa, M. A.; deGroot, K. J. Mater. Sci.: Mater. Med. 1997, 8, 423-426. (21) Ramqvist, L.; Hamrin, K.; Johansso, G.; Fahlman, A.; Nordling, C. J. Phys. Chem. Solids 1969, 30, 1835-1847. (22) Hanawa, T.; Ota, M. Appl. Surf. Sci. 1992, 55, 269-276. (23) Kuznetsov, M. V.; Zhuravlev, J. F.; Gubanov, V. A. J. Electron Spectrosc. Relat. Phenom. 1992, 58, 169-176. (24) Ikeo, N.; Iijima, Y.; Niimura, N.; Sigematsu, M.; Tazava, T.; Matsumoto, S.; Kojima, K.; Nagasawa, Y. Handbook of X-ray photoelectron spectroscopy JEOL: Tokyo, Japan, 1991. (25) Porte-Durrieu, M. C.; Labrugere, C.; Villars, F.; Lefebvre, F.; Dutoya, S.; Guette, A.; Bordenave, L.; Baquey, C. J. Biomed. Mater. Res. 1999, 46, 368-375. (26) Wagner, C. D.; Riggs, W. M.; Davis, L. E.; Moulder, J. F. Handbook of X-ray photoelectron spectroscopy; Mulenberg, G. E., Ed.; Perkin Elmer Corp: Eden Prairie, MN, 1979. (27) Barr, T. L. J. Vac. Sci. Technol., A 1991, 9, 1793-1805.
The surface free energy components (polar and dispersive) were calculated through the geometric mean approach7 (based on Young’s equation and eq 2). Table 2 presents the values of the surface free energy of the Ti substrates (γSV) and the dispersive (γdSV) and polar (γpSV) components as well as the polarity. The polarity is defined as the ratio between the polar component divided by the total surface free energy (γpSV/γSV). All substrates are predominantly dispersive, although the Ti substrates after H2O2 treatment have a higher contribution of the polar component due to the presence of ionic species. The surface free energy increases after H2O2 treatment, as there are more reactive sites exposed from the oxide. Considering that polarity is a quantitative indicator of hydrophilicity, we can say that the TiO2 sputtered substrate is the more hydrophobic substrate. Albumin Adsorption. XPS. Wide scans were performed on TiO2 cp and TiO2 sp surfaces, and the composition and morphology of the spectra are identical for both surfaces. For illustration only, the data on the TiO2 cp surfaces are shown (Figures 2-4). Ti, O, C, N, P, and Ca were always present. S was present for HSA concentrations >0.30 mg/mL. Ca and P have their origins in the electrolyte and C, N, O, and S in the protein. The surface composition of Ti samples has been extensively reported,20,22,28-30 but only a few have deconvoluted and assigned each peak (C1s or N1s) to the protein bonds.31-33 In this work, we also followed the atomic % of each element during kinetics of adsorption as well as adsorption isotherms. High-resolution spectra were acquired for Ti2p, O1s, C1s, N1s, S2p, Ca2p, and P2p, providing an indication of the chemical composition of the titanium oxide and protein film formed at the surfaces. The C1s spectrum of albumin is significantly different from that of a TiO2 surface. A C1s peak broadening was observed after protein adsorption. It was considered that the C1s peak had a contribution of four different peaks corresponding to carbon atoms in different environments, that is, to saturated hydrocarbon groups (sCH3, sCH2s) with a BE of 285.0 eV, to amine groups (sCsNHs) with a BE of 286.6 eV, to the peptide bond (sCdOsNHs) with a BE of 288.2 eV, and to acidic groups (sCsCOO-) with a BE of 289.6 eV.32 Figure 2a shows an envelope for the C1s deconvolution peak after HSA adsorption ([HSA] ) 0.20 mg/mL), with the sCH2s groups being the major contribution to the C1s intensity. The kinetics of albumin adsorption on titanium samples could be followed by the C1s peak intensity. Figure 3a shows that as the time of albumin incubation increases the peak intensities also increase. (28) Wa¨livaara, B.; Aronsson, B. O.; Rodahl, M.; Lausmaa, J.; Tengvall, P. Biomaterials 1994, 15, 827-834. (29) Oji, M. O.; Wood, J. V.; Downes, S. J. Mater. Sci.: Mater. Med. 1999, 10, 869-872. (30) Pan, J.; Liao, H.; Leygraf, C.; Thierry, D.; Li, J. J. Biomed. Mater. Res. 1998, 40, 244-256. (31) Ratner, B. D.; Horbett, T. A.; Shuttleworth, D.; Thomas, H. R. J. Colloid Interface Sci. 1981, 83, 630-642. (32) Lindberg, B.; Maripuu, R.; Siegbahn, K.; Larsson, R.; Golander, C. G.; Eriksson, J. C. J. Colloid Interface Sci. 1983, 95, 308-321. (33) Auditore, A.; Satriano, C.; Coscia, U.; Ambrosone, G.; Parisi, V.; Marletta, G. Biomol. Eng. 2002, 19, 85-90.
HSA Adsorption on TiO2
Langmuir, Vol. 20, No. 22, 2004 9749 Table 2. Contact Angles and Their Standard Deviations of Water and Diiodomethane (n ) 10) on TiO2 Surfaces at t ) 0 sa TiO2 sp
Ti cp (before H2O2 treatment)
TiO2 cp (after H2O2 treatment)
p γSV , mN/m
84 ( 2 52 ( 2 36.3 3.53
74 ( 3 53 ( 2 39.5 7.30
71 ( 3 49 ( 3 42.7 8.17
d γSV , mN/m
p γSV /γSV
θwater, deg θdiiodomethane, deg γSV, mN/m
a The values of the surface free energy of the TiO substrates 2 and their dispersive and polar components and the polarity are also shown.
Figure 2. Representative deconvolution of the XPS envelope for (a) N1s, (b) C1s, and (c) O1s peaks (after 60 min of 0.20 mg/mL HSA adsorption at a TiO2 cp surface) at 0°.
Figure 1. 3D AFM images of a (a) TiO2 sputtered surface, (b) Ti cp surface (before H2O2 treatment), and (c) TiO2 cp surface (after H2O2 treatment).
Figure 4a presents the variation of C%, assigned to each component, as a function of albumin concentration in solution. A plateau is attained between 0.30 and 1.0 mg/ mL HSA in solution.
The N1s spectra, after albumin adsorption, were considered to have a contribution of three different peaks corresponding to sNH3+ with a BE of 401.8 eV, to the peptide bond (sCdOsNHs) with a BE of 400.1 eV, and to the NH2 groups with a BE between 389.9 and 399.9 eV32,33 (Figure 2b). The neutral peptide nitrogen peak dominates the N1s spectrum, contributing more than 90% to the total amount. Figure 3b shows that the intensity of the N1s peak clearly increases due to albumin adsorption on TiO2 cp after 5 min of protein incubation. As the time of incubation increases, the quantity of albumin
Langmuir, Vol. 20, No. 22, 2004
Figure 3. Evolution of the XPS element envelope with increased time of albumin immersion ([HSA] ) 0.20 mg/mL).
adsorbed to the TiO2 cp surface also increases, attaining a maximum value for 60 min of adsorption. The N% (peptide bond) reaches a semiplateau for lower HSA concentrations (0.30 mg/mL), with the peptide bond being the main contribution for the total N (Figure 4b). The shape of the O1s peak after protein adsorption is similar to the one without protein, suggesting that the contributions from the carboxyl groups and the phosphate from the electrolyte are superimposed on the OH peak. Upon adsorption, the OM% decreases and the OH% increases, indicating that a film of protein is covering the titanium oxide (Figure 4c). As expected, the increasing exposure to albumin resulted in a protein layer covering the TiO2, as indicated by the decrease of the Ti signal (Figure 3c) as well as by the increase of the N1s and C1s intensity. The atomic percentages of Ti, OM, and OH versus [HSA] are shown in Figure 4c. As the concentration of the albumin solution increases, the Ti% and the OM% decrease and the OH% increases, attaining a semiplateau between 1.0 and 4.0 mg/mL, due to the existence of a protein layer. Only one peak is observed in the high-resolution S2p spectra, resulting from the sulfur atoms coming from the disulfide groups (-S-S-) in protein molecules at 164.1 eV.32 P is present as a trace element arising from the electrolyte solution. Wettability Studies. To have further data on protein adsorption, wettability studies were performed and the work of adhesion between the protein solutions and the surfaces was calculated from the values of the contact angles and the surface tensions of the protein solutions through eq 2.
Sousa et al.
Figure 4. Changes in atomic % with [HSA] in solution after 60 min of adsorption at a TiO2 cp surface: (a) C%; (b) N%; (c) Ti% and O%.
Figure 5. Time dependence contact angle of several solutions at a TiO2 cp surface.
A decrease in the contact angle versus time is observed for the different albumin solutions at the TiO2 surfaces (Figure 5, for the TiO2 cp). The variation is more pronounced for the plasma solutions. These solutions are complex mixtures of several proteins and ions, and therefore, the migration of these species to the drop boundary is delayed relative to the single protein solution. The values of the contact angles of protein solutions for the TiO2 substrates, given in Table 3, were obtained by extrapolation of time-dependent experimental results to t ) 600 s. The contact angles of HSA with TiO2 cp are not dependent on albumin concentration (Table 3), since they are not statistically different. Comparing the two surfaces, the contact angle of a HSA solution with 4.0 mg/mL follows an identical trend to the contact angle between the surfaces and water. When a plasma solution was assayed, a higher
HSA Adsorption on TiO2
Langmuir, Vol. 20, No. 22, 2004 9751
Table 3. Contact Angles and Their Standard Deviation of PBS and Different Protein Solutions on TiO2 Surfaces at t ) 600 s a θ, deg solution
TiO2 cp (after H2O2 treatment)
PBS 0.02 mg/mL HSA 0.20 mg/mL HSA 4.0 mg/mL HSA plasma 10% plasma
72.9 ( 0.20 58.0 ( 0.48 56.0 ( 0.48 53.4 ( 0.70 50.1 ( 0.49 47.0 ( 0.33
77 ( 3 64 ( 2 65 ( 3 70 ( 2 52 ( 2 42 ( 4
76 ( 4 62 ( 3 63 ( 4 65 ( 4 57 ( 3 49 ( 3
The surface tension of the liquids (γLV) is also shown.
affinity of the solution to the TiO2 cp surface was also observed. The surface tension of the different solutions was measured. The surface tension of PBS stays constant during the time of the experiment. The protein solutions have lower surface tensions, which decrease rapidly within the first 100-200 s, reaching then a plateau or a semiplateau (data not shown). Several authors attribute this behavior to the adsorption of protein molecules to the air-solution interface.34,35 This is clearer for the plasma solutions, as a consequence of the higher concentration of proteins. The surface tensions of different protein solutions (t ) 600 s) are shown in Table 3. Measurements of the time-dependent contact angles and liquid surface tensions combined with the knowledge of the solid surface free energy, assumed to be time independent, may be used to estimate dynamic solidliquid interfacial tensions according to Young’s equation. However, since the application of Young’s equation to a nonequilibrium process is not straightforward, care should be taken in the interpretation of the results.36,37 The time dependence of the work of adhesion between each protein and TiO2 was then evaluated through the Young-Dupre´ equation, from the correspondent values of γLV and θ. The advantage of measuring the work of adhesion relies on the fact that this parameter can be measured at any instant of time, whether the system is in equilibrium or not, and correctly interpreted as the force needed to separate the liquid from the substrate.38 To understand the influence of the presence of a protein on the behavior of the solid-liquid interface, we compared the work of adhesion of the water with the work of adhesion of albumin and of the plasma solution (Figure 6). As expected from the surface free energy values, the work of adhesion of water is higher on the TiO2 cp substrate than on the TiO2 sp substrate (Figure 6a). Analysis of the three parts of Figure 6 shows that the work of adhesion of the protein solutions follows the same trend. The cp surface is the one presenting the highest value of the work of adhesion for all solutions (Figure 6), implying a high solid-liquid interaction.38 Adsorbed macromolecules may use several adsorption sites depending on their structure and molecular mass. At low concentrations, adsorbed proteins are in an unfolded state. At higher protein concentrations, the adsorption layer becomes more compressed and molecules (34) Miller, R.; Treppo, S.; Voigt, A.; Zingg, W.; Neumann, A. W. Colloids Surf. 1993, 69, 203-208. (35) Serro, A. P. V.; Fernandes, A. C.; Saramago, B. D. V. Colloids Surf., A 1997, 125, 209-219. (36) Lopes, M.; Monteiro, F.; Santos, J.; Serro, A.; Saramago, B. J. Biomed. Mater. Res. 1999, 45, 370-375. (37) Ferraz, M. P.; Monteiro, F. J.; Serro, A. P.; Saramago, B.; Gibson, I. R.; Santos, J. D. Biomaterials 2001, 22, 3105-3112. (38) Vogler, E. A.; In Wettability; Berg, J. C., Ed.; Surfactant science series 49; Marcel Dekker: New York, 1993; pp 183-250.
Figure 6. Work of adhesion between TiO2 substrates and (a) water, (b) [HSA] ) 4.0 mg/mL, and (c) plasma.
Figure 7. Work of adhesion between TiO2 cp and HSA at different concentrations and between TiO2 cp and plasma solutions.
with different degrees of unfolding will coexist at the interface.34 These phenomena can perhaps explain the highest work of adhesion for the lowest HSA concentration (Figure 7). Although the work of adhesion cannot be seen as a direct measure of protein adsorption, it quantifies the decrease in surface free energy due to protein adsorption.37 Our results indicate a linear relation between the work of adhesion and the logarithm of the albumin concentration (Figure 8). The work of adhesion between plasma and TiO2 cp is opposite to the one found for the albumin solutions (Figure 7), that is, higher for the undiluted solution. 125 I-HSA Radiolabeling. The amount of iodide ion adsorbed to a titanium surface after exposure to unlabeled protein plus labeled free iodide was found to be ∼0.2%.
Langmuir, Vol. 20, No. 22, 2004
Figure 8. Work of adhesion between HSA molecules and the TiO2 substrates as a function of HSA concentration in solution (t ) 600 s).
Sousa et al.
Figure 11. Comparison of the kinetics of HSA adsorption (0.20 and 4.0 mg/mL) and desorption (with HSA) from a TiO2 cp surface.
Figure 9. HSA adsorption isotherms for TiO2 substrates after 1 h of incubation. Figure 12. Comparison of the kinetics of HSA adsorption (0.20 and 4.0 mg/mL) on TiO2 sp and desorption (with HSA).
Figure 10. Elution of HSA by other HSA molecules from TiO2 cp and TiO2 sp as a function of HSA concentration in solution. The elution time was 24 or 72 h for the TiO2 cp and 24 h for the TiO2 sp.
This amount is negligible, considering that in our solution we only have ∼2% free iodide ions, instead of 100%, and that only 0.2% of the free iodide can adsorb to our substrate. This result justifies the use of a buffer without nonlabeled iodide ion, PBS. Preferential adsorption of the 125I-labeled albumin did not occur on the TiO2 cp surface, as determined by varying the ratio of labeled to unlabeled protein in a series of control experiments. The total HSA concentration was 1.0 mg/ mL, as determined by the bicinchoninic acid (BCA) assay. The amount of HSA adsorbed in all experiments to TiO2 cp was 5.0 mg/m2. Using HSA concentrations between 0 and 10 mg/mL for the TiO2 sp surface and between 0 and 4.0 mg/mL for the TiO2 cp surface, adsorption isotherms were performed (Figure 9). The adsorbed amount increased with HSA concentration, and a plateau is reached for concentrations of ∼1.0 mg/mL for TiO2 cp and ∼4.0 mg/mL for TiO2 sp. After the adsorption step from single HSA solutions, desorption was performed with HSA (10.0 mg/mL) washes for periods of 24 and 72 h, to evaluate the exchangeability of adsorbed HSA molecules by HSA in solution. The HSA molecules adsorbed on TiO2 sp seem to be more easily exchanged by HSA itself (Figure 10) than those adsorbed on TiO2 cp after 24 h, since 60-65% of HSA is eluted from the TiO2 sp surface and only 20-30% of adsorbed protein
was desorbed from the TiO2 cp surface. In contrast, after 72 h, nearly all the adsorbed albumin molecules effectively exchange with other albumin molecules from the TiO2 cp surface. The initial protein concentration in solution does not influence HSA exchangeability, for both substrates, since identical elutions are obtained for 0.20 and 4.0 mg/mL (after 24 and 72 h). The kinetics of albumin adsorption was studied on TiO2 surfaces. Figures 11 and 12 show that rapid HSA adsorption takes place on both surfaces. Nevertheless, for the time period studied, the albumin adsorption on both TiO2 surfaces increased steadily to ∼60 min of incubation. Figures 11 and 12 show the kinetics of HSA adsorption at two different concentrations, 0.20 and 4.0 mg/mL, and subsequent desorption with HSA. For the lower HSA concentration in solution, as the time of incubation increases, the albumin desorbed also increases. For the higher concentration in solution, after 60 min of immersion, desorption was at a minimum. For both albumin concentrations, there are practically no exchanged HSA molecules. Discussion The influence of the nature of titanium oxide and of its hydrated state, as well as of the surface on biocompatibility, has become an important area of research.4,39-41 It has been shown that the method of preparation of titanium oxide has an effect on the dissolution behavior of this material in biological environments29,42,43 and consequently on its in vivo performance.44 (39) Feng, B.; Weng, J.; Yang, B. C.; Qu, S. X.; Zhang, X. D. Biomaterials 2003, 24, 4663-4670. (40) Morra, M.; Cassinelli, C.; Cascardo, G.; Cahalan, P.; Cahalan, L.; Fini, M.; Giardino, R. Biomaterials 2003, 24, 4639-4654. (41) Wa¨livaara, B.; Lundstrom, I.; Tengvall, P. Clin. Mater. 1993, 12, 141-148. (42) Lincks, J.; Boyan, B. D.; Blanchard, C. R.; Lohmann, C. H.; Liu, Y.; Cochran, D. L.; Dean, D. D.; Schwartz, Z. Biomaterials 1998, 19, 2219-2232.
HSA Adsorption on TiO2
Langmuir, Vol. 20, No. 22, 2004 9753
In this study, we prepared two simple titanium oxides, one sputtered on Si (TiO2 sp) and another by Ti immersion in 10 mM H2O2 solution for 48 h (TiO2 cp). The latter treatment conditions were selected among other hydrogen peroxide concentrations and times of immersion. XPS reveals that both treatments led to a regular and uniform layer of TiO2, without suboxides such as TiO and Ti2O3, sufficiently thick to prevent the emission of photoelectrons from the bulk material to the surface. Regarding the Ti/O ratio data, the Ti/OM ratio assumes values near the theoretical (1/2). As expected, the Ti/OH ratio assumes higher values near the interface for the TiO2 cp substrate due to the existence of a hydrated film. Tengvall et al.4 reported that titanium surfaces treated with H2O2 (130%) showed that the surface Ti/OM ratio decreases when immersed in solutions of up to 10 mM H2O2, that is, in agreement with the data obtained in this work. In addition, the TiO2 film is thicker in 10 mM H2O2 than in 100 mM H2O2,41 which corroborates our choice of the peroxide concentration. The two TiO2 surfaces have distinct roughnesses, with the TiO2 sp having a mean Ra value 14 times smaller than the one for the TiO2 cp (Figure 1). Wenzel was one of the first investigators to propose a model relating contact angles and surface roughness.45 Roughening a substrate usually decreases its wettability,46 which is in agreement with the results obtained here. Moreover, the increased surface energy observed in H2O2-treated surfaces is also indicative of higher wettability.41 All substrates are predominantly dispersive, although the Ti substrates after H2O2 treatment have a higher contribution of the polar component due to the presence of ionic species. The surface free energy increases after H2O2 treatment as a result of the existence of more reactive sites exposed on the oxide layer. Considering that polarity is a quantitative indicator of hydrophilicity, we can say that the TiO2 sputtered substrate is the more hydrophobic one. Concerning protein adsorption, contact angle determination revealed a decrease in the contact angles as time increased for the different albumin solutions at both TiO2 surfaces (Figure 5 for TiO2 cp). The variation is more pronounced for the plasma solutions. These solutions are complex mixtures of several proteins and ions, and therefore, the migration of these species to the drop boundary is delayed relative to the single protein solution. Rakhorst et al.47 showed that plasma did not influence the initial contact angle at HDPE, PDMS, PTFE, and PU. The more accentuated decrease of the contact angles was correlated with higher levels of albumin and fibrinogen adsorption as well as platelet adhesion. These authors refer to the biocompatibility properties of the tested materials that might be related to the time behavior of the contact angles in time, rather than to the initial hydrophobic or hydrophilic state. However, some precaution on the interpretation of biocompatibility based on hydrophilic/hydrophobic interactions should be taken. If the above hypothesis were always true, it would be expected that TiO2 cp presents higher levels of albumin adsorption than TiO2 sp, since the former surface shows
a higher change in contact angle of plasma (∆θ ) -23° (t ) 600 s)) than the latter surface (∆θ ) -18° (t ) 600 s)). This conclusion as well as the contact angle after 600 s (Table 3) is apparently in disagreement with the results obtained by 125I-HSA radiolabeling. The radiolabeling data were expressed as the ratio between the amount of adsorbed protein and the geometric area. If the real area was considered, a higher difference would be observed, since the TiO2 cp surface is rougher than the TiO2 sp surface. The quantity of albumin adsorbed is higher on the more hydrophobic surface (TiO2 sp) which is in agreement with the hypothesis defended in the literature by many authors48-51 that hydrophobic surfaces generally adsorb more albumin than hydrophilic surfaces. The hydrophilicity of a metal surface could be an important factor in determining protein adsorption, but there may also be other factors relevant for metal surfaces which are not important for polymer surfaces, namely, surface charge and chemical binding between the metal and the protein.52 Both TiO2 surfaces have almost the same surface composition, but the chemically polished titanium after peroxide treatment presents more OH- groups than the sputtered titanium oxide (Ti/OH ) 0.77 or 1.1, respectively), conferring to the former surface a higher negative charge. At physiological pH, albumin has also a net negative charge that repels the TiO2 cp surface. Although the work of adhesion cannot be seen as a direct measure of protein adsorption, it quantifies the decrease in interfacial free energy (γSL) due to protein adsorption.37 The wettability results also showed that the work of adhesion of HSA to TiO2 cp decreased linearly as the albumin concentration increased. Macromolecules adsorbed can use several adsorption sites depending on their structure and molecular mass. At low concentrations, adsorbed proteins are in an unfolded state with more located binding sites to adsorption. It is known53,54 that the driving forces for the adsorption of “soft” proteins such as HSA are related to structural rearrangements in the molecules that enable them to overcome the unfavorable conditions offered by an electrostatically repelling surface. At higher protein concentrations, the adsorption layer becomes more compressed and molecules with different degrees of unfolding will coexist at the interface,34 being more difficult or maybe impossible for some molecules to overcome the unfavorable conditions to adsorption. These phenomena can perhaps explain the highest work of adhesion obtained for the lowest HSA concentration observed (Figure 4). The opposite correlation was found for the plasma and TiO2 cp substrate (Figure 7). This behavior may result from a simultaneous adsorption of other plasma proteins with albumin (namely, adhesion proteins such as fibronectin and vitronectin) or exchanged with albumin molecules that are in a higher concentration at undiluted plasma and have a higher affinity to the surface. The work of adhesion of both 4.0 mg/mL HSA and plasma is higher for TiO2 cp than for TiO2 sp which may be correlated with the higher polar component of the surface free energy of TiO2 cp.
(43) Ong, J. L.; Carnes, D. L.; Cardenas, H. L.; Cavin, R. Implant Dent. 1997, 6, 19-24. (44) Ricci, J. L.; Spivak, J. M.; Blumenthal, N. C.; et al. In The bone biomaterial interface; Davis, J. E., Ed.; University of Toronto Press: Toronto, 1991; pp 334-349. (45) Busscher, H. J.; Vanpelt, A. W. J.; Deboer, P.; Dejong, H. P.; Arends, J. Colloids Surf. 1984, 9, 319-331. (46) Hitchcock, S. J.; Carroll, N. T.; Nicholas, M. G. J. Mater. Sci. 1981, 16, 714-732. (47) Rakhorst, G.; Van der Mei, H. C.; Van Oeveren, W.; Spijker, H. T.; Busscher, H. J. Int. J. Artif. Organs 1999, 22, 35-39.
(48) Martins, M. C.; Ratner, B. D.; Barbosa, M. A. J. Biomed. Mater. Res. 2003, 67A, 158-171. (49) Sigal, G. B.; Mrksich, M.; Whitesides, G. M. J. Am. Chem. Soc. 1998, 120, 3464-3473. (50) Prime, K. L.; Whitesides, G. M. Science 1991, 252, 1164-1167. (51) Vandulm, P.; Norde, W. J. Colloid Interface Sci. 1983, 91, 248255. (52) Williams, R. L.; Williams, D. F. J. Colloid Interface Sci. 1988, 126, 596-603. (53) Serro, A. P. V. A.; Fernandes, A. C.; Saramago, B. D. V.; Norde, W. J. Biomed. Mater. Res. 1999, 46, 376-381. (54) Norde, W.; Anusiem, A. C. I. Colloids Surf. 1992, 66, 73-80.
Langmuir, Vol. 20, No. 22, 2004
Figure 13. Comparison between adsorption of albumin onto a TiO2 cp surface by 125I-HSA radiolabeling and XPS measurements of N%.
Radiolabeling of albumin has shown that the adsorbed amount increases with HSA concentration and a plateau is reached for concentrations of ∼1.0 mg/mL for TiO2 cp. As shown in Figure 13, the same conclusion may be drawn from the evolution of the N% determined by XPS. Thus, XPS can be successfully used as an alternative technique to study isothermal adsorption of albumin, correlating well with 125I-labeled HSA data. Although proteins often adsorb as monolayers, multilayer adsorption is not uncommon, namely, for highconcentration solutions.55,56 Knowing the size of the protein molecule and the molecular mass, it is possible to estimate the surface occupied by the molecules lying perpendicular or parallel to the surface and to convert it to the mass of albumin per unit surface (m2). The theoretical values for closely packed monolayers formed by side-on adsorption and end-on adsorption are 2.14 and 7.90 mg/m2, respectively. By comparison with the data obtained by 125IHSA (Figure 9), these values suggest that the albumin adsorption on both TiO2 substrates is a multilayer coverage. Regarding the exchangeability with other albumin molecules, the HSA molecules adsorbed on TiO2 sp seem to be more easily exchanged (Figure 10) than those adsorbed on TiO2 cp after 24 h, since 60-65% of HSA is eluted from the TiO2 sp surface and only 20-30% of adsorbed protein was desorbed from the TiO2 cp surface. This result is expected if we look for the work of adhesion for both substrates; that is, HSA molecules are less tightly bound at hydrophobic surfaces than at hydrophilic surfaces. It is expected that, at least in aqueous media, nonpolar interactions are stronger than polar interactions;57 however, the binding strength seems to be at a maximum if both polar and nonpolar interactions are (55) Young, B. R.; Pitt, W. G.; Cooper, S. L. J. Colloid Interface Sci. 1988, 125, 246-260. (56) Feng, L.; Andrade, J. D. Biomaterials 1994, 5, 323-333. (57) Norde, W. Adv. Colloid Interface Sci. 1986, 25, 267-340.
Sousa et al.
involved, as is the case for the TiO2 cp substrate. Besides, Kurral et al.58 and Martins et al.48 suggested that the main mode of interaction of HSA onto hydroxylated metals was via hydrogen bonds. Although hydrogen bonds are individually weak, the probability of breaking many hydrogen bonds simultaneously is low. This can be responsible for changing the adsorption behavior of the protein from reversible to “irreversible”. However, after 72 h, nearly all the adsorbed albumin molecules effectively exchange with other albumin molecules at the TiO2 cp surface. According to Brash et al.,59 the exchange of albumin is slow, ∼40 h, and as the surface-protein interactions are stronger for the TiO2 cp substrate, a longer time is necessary for the total exchange. For the higher concentration in solution and for both substrates, as the time of incubation increases it is notorious that albumin exchangeability diminishes perhaps due to conformational changes. Conclusions Two simple titanium oxides were prepared, one sputtered on Si (TiO2 sp) and another obtained by Ti immersion in 10 mM H2O2 solution for 48 h (TiO2 cp). XPS revealed that both treatments led to a regular and uniform layer of TiO2, without suboxides such as TiO and Ti2O3, sufficiently thick to prevent the emission of photoelectrons from the bulk material to the surface. The two TiO2 surfaces have distinct roughnesses, with the TiO2 sp having a mean Ra value 14 times smaller than the one for TiO2 cp. TiO2 cp adsorbs less albumin than TiO2 sp, as shown by the radiolabeling data, but the adherent molecules are strongly attached to the former surface, as indicated by the work of adhesion and by the desorption studies. The data obtained by 125I-HSA also suggest that albumin adsorbs as a multilayer. Isothermal and kinetics of albumin adsorption on titania surfaces can be successfully studied by XPS and by 125IHSA radiolabeling measurements, and both techniques correlate well. Acknowledgment. The authors would like to thank Doctor Paulo Freitas and Doctor Susana Freitas (INESC) for the titanium oxide sputtered sample preparation, Doctor Carlos Sa´ (CEMUP) for assistance in the XPS investigation, and the Portuguese Institute of Blood (IPS) for donating the human plasma samples. LA049158D (58) Kurrat, R.; Prenosil, J. E.; Ramsden, J. J. J. Colloid Interface Sci. 1997, 185, 1-8. (59) Brash, J. L.; Uniyal, S.; Samak, Q. Trans. Am. Soc. Artif. Intern. Organs 1974, 20A, 69-76.